Localization of acoustic modes in periodic porous silicon structures
© Lazcano et al.; licensee Springer. 2014
Received: 12 May 2014
Accepted: 4 July 2014
Published: 21 August 2014
The propagation of longitudinal acoustic waves in multilayer structures based on porous silicon and the experimental measurement of acoustic transmission for the structures in the gigahertz range are reported and studied theoretically. The considered structures exhibit band gaps in the transmission spectrum and these are localized modes inside the band gap, coming from defect layers introduced in periodic systems. The frequency at which the acoustic resonances appear can be tuned by changing the porosity and/or thickness of the defect layer.
KeywordsPorous silicon Localized defects Phononic crystals Acoustic transmission
The study of acoustic and elastic wave propagation in phononic crystals (PCs) [1–3] have been studied theoretically  and experimentally  in recent years. In analogy with the photonic band gap materials, emphasis in phononic crystals has been on achieving large acoustic band gaps within which propagation of sound is forbidden.
The interest about phononic band gap materials is in both, pure and applied physics. Fundamental physics has a special interest concerned with the localization phenomena of sound and vibrations in PCs. Researchers have prospected numerous applications based on cavity structures built around PCs, such as wave filters, waveguides, and splitters [6–9]. Furthermore, it is possible to design cavities for coherent (single-wavelength) phonon generation and control, to attain phonon amplification and ‘lasing’ in the called ‘saser’, one of the most important potential applications [10–12].
Periodic solid-state structures exhibit transmission stop bands for waves at certain frequencies. By placing one or more defects into a perfect phononic crystal, acoustic cavities are created inside the system. The presence of these defects, produces localization of elastic or acoustic modes inside the phononic band gap. These localized modes are the acoustic analog of donor or acceptor states produced inside the band gap of semiconductors. In analogy with electronic systems, one can consider these acoustic states to control the sound propagation through the structure.
If a defect is introduced into a periodic structure, the translational symmetry is broken and highly localized defect modes within the band gaps are created [6, 8, 13, 14]. Point, linear, and planar defect states have been theoretically investigated in one-dimensional (1D), two-dimensional (2D), and three-dimensional (3D) phononic crystals [3, 15, 16]. In 1D structures, a microcavity can be a spacer layer of thickness λ/2 enclosed by two Bragg reflectors . In 2002, Trigo et al. proposed phonon cavities in structures consisting of two semiconductor superlattices enclosing a spacer layer, showing that acoustical phonons can be confined in such layered structures if the spacer thickness is an integer multiple of the acoustic half-wavelength at the center of one of the superlattice-folded minigaps. These acoustic cavities are semiconductor multilayers in the nanometer scale and are fabricated by molecular beam epitaxy (MBE), which is a sophisticated and expensive technique that requires ultra-high vacuum system and a very tight control on the growth parameters, and modulate the thicknesses is easier than to modulate the elastic properties of the layers. Contrasting, porous silicon (PS) multilayer fabrication is relatively easy and considerably less costly, besides that this material allows to modulate both the thicknesses and the elastic properties of each layer.
PS is known as a versatile material with applications in light emission, sensing, and photonic devices . The possibility of producing acoustic band gaps in PS was proposed in 2005 , and detailed calculations of predicted bandwidths were subsequently published . Recently, experimental results of Brillouin light scattering suggested the existence of zone-folded phonons and phononic band gaps in PS multilayers . G. N. Aliev et al. in 2010 reported experimental measurements of transmission for longitudinal acoustic waves and observation of hypersonic band gaps in a periodic PS structure with an acoustic microcavity consisting of a spacer layer of thickness λ/2 .
By taking advantage of the possibility to modulate the elastic properties of PS layers, and considering that it is possible to create localized modes by introducing a defect layer with different acoustic properties into a periodic structure, in this paper, we investigate the propagation of longitudinal acoustic waves in multilayer structures based on PS, that exhibit resonant cavity modes in frequencies of gigahertz (GHz), consisting of defect layers intentionally introduced in periodic structures. The design and material parameters that allow to create these localized acoustic modes is discussed, and experimental results of the measured acoustic transmission in PS samples fabricated by electrochemical etching are presented.
The multilayer PS structures studied here have thicknesses in micrometer range and the procedure used to fabricate them creates mesoporous silicon with an average pore diameter of 20 to 50 nm. On the other hand, in our experiments, the typical longitudinal wavelengths excited throughout the samples are 3 to 7 μ m depending on porosity. Accordingly, each of the individual layers in the structures is assumed to be homogeneous.
where ρ j is the mass density, and u(z,t) is the atomic displacement. Here, j is an index identifying each layer. The limits of the elastic continuum description of wave propagation in ordered media depends on the dimensions of the system compared with the wavelength. When the dimensions approach nanometer-length scales, atomistic treatments using first principles or semi-empirical methods may become necessary . However, in our case, the thicknesses of the layers are in the micrometer range and each layer can be considered as a homogeneous layer; thus, the model described before is assumed valid.
In a solid, the acoustic waves can be longitudinal or transversal. In this letter, only longitudinal waves propagating through PS are considered because in our experiments, the waves are coupled to the samples through a liquid at normal incidence. The mass density ρ is a function of the porosity and is described by ρ=ρ0(1−P) where ρ0=2.330 g/cm 3 is the density of bulk silicon and P the porosity. The acoustic velocity dependence on porosity is given empirically by v L =vL 0(1−P) k , being vL 0 the longitudinal velocity of sound in bulk silicon along the (100) crystallographic direction and k≥0.5 is a constant [25–28]. In general, the parameter k depends on PS morphology which in turn depends on the doping level of the Si substrate [25, 26].
If we consider a structure formed by N layers, the total transfer matrix representing the structure is obtained by multiplying, in the appropriate order, a series of N transfer matrices, each one given by a matrix of the type appearing in Equation 6. The obtained matrix relates the displacement vector at the beginning of the structure with that at the end, and represents a 2 × 2 set of equations that can be fully solved.
With the above formalism, one can derive the acoustic eigenenergies and eigenvectors. The reflectivity and transmission can also be calculated as the square modulus of and , respectively, by imposing the boundary conditions and for a wave traveling from right to left. Here 0 and N label the first and last layer of the structure, respectively.
Attenuation can be included by taking the wave vector k j complex, such that K j =k j −α i , where α i is attenuation coefficient. The form of the attenuation coefficient depends on the physical process causing loss and we assume that the Akhiezer model is dominant in a semiconducting material. This gives α=η ω2/2ρ v3, where η is the viscosity. However, it is known that introducing acoustic attenuation into the model leads to important effects as the shrinking of gaps, only for frequencies higher than 180 GHz ; therefore, no absorptive behavior is considered in our model since no important effects are obtained if they are included.
Furthermore, the position and width of the band gap are critical parameters for devices that reflect or localize the acoustic waves . Band structures of many kinds of periodic phononic crystals have been reported [31–33]. The most commonly studied acoustic band gaps in 1D PCs are the Bragg type, appearing at an angular frequency ω of the order of vL(T)/d (vL(T) refers to the longitudinal (transverse) elastic wave velocity and d is the lattice constant).
In , the authors considered periodic semiconductor structures of GaAs/AlAs to introduce microcavities as spacer layers of thickness λ/2. However, for a 10-period GaAs/AlAs mirror, R B ∼0.880, while R B ∼0.996 if n=20. For a PS structure, a porosity variation of 15 % between the constituent layers of 52 % and 67 % of porosity, leads to R B ∼0.997 for n=6. Thus, by modulating the porosity of the PS structures, very high reflectivity values can be achieved. This is an essential condition to obtain narrow transmission bands into the stop bands corresponding to the cavity modes.
where u(z,f) is the displacement field distribution at each frequency, which is obtained by the transfer matrix method.
Samples were electrochemically etched from boron-doped (100)-oriented Si substrates with a resistivity of 0.007 to 0.013 Ω cm. Room-temperature anodization was performed using a 1:1 solution of HF (40 %) and ethanol (99.98 %). The acoustic transmission measurements reported here were done using a Vector Network Analyzer (VNA). Each sample was placed between two ZnO-based piezoelectric transducers with a central frequency of 1.1 GHz and an operation bandwidth of 500 MHz. The transducers consist of a piezoelectric layer driving waves into a silicon pillar with a thickness of 520 μ m. To couple the transducers to the specimen, In-Ga eutectic was used. The transducer front surface was aligned parallel to the sample surface using two orthogonal microscopes so that the acoustic waves impinge normally into the PS layers. The transducers were connected to the VNA ports and transmission parameters were measured as function of frequency, more details of the experimental set-up can be found in . Dependence of sound velocity with porosity for Si wafers and experimental conditions used here were determined previously and reported in , the values of vL 0 and the parameter k used here are 8.44 km/s and 0.56, respectively.
For the fabrication of PS multilayers, we consider the inclusion of ‘etch stops’ or ‘etch breaks’ where the current is interrupted to stop the etching of the Si wafer in order to prevent any depletion of HF . The introduction of these etching breaks is necessary to obtain layers with constant porosity with depth . Because our samples include very thick layers, with large mismatch porosities between them, the number and length of the etch breaks are important to obtain homogeneous structures. We found that etch breaks of 4 s with a ratio (etch break time)/(etching time) from 3.3 for low porosities (52 %) to 7.3 for high porosities (67 %) are enough to minimize any chirp in the layers.
Results and discussion
Thicknesses of layers were measured by optical microscopy, and the layer porosities were determined from optical reflectance spectra by fitting our experimental measurements and comparing them with our theoretical simulations for each sample. The acoustic transmission and field intensity distribution have been modeled using the transfer matrix method described before and taking into account the effect of the sample (PS-Si substrate), transducers (Si pillars), and In-Ga eutectic liquid used to couple the transducers to the sample.
Now, based on the concepts mentioned before about cavities, we will show how the intentional introduction of a defect layer between a pair of mirrors can lead to formation of an acoustic cavity mode within the stop band. For this purpose, we consider two structures: sample 2 and sample 3.
The modeled transmittance of the periodic case (sample 1) and for the two cavity structures (samples 2 and 3), obtained by the TMM, shows a good match with the experimental results. The localized acoustic resonances can be tuned at different frequencies (within the acoustic band gap) by changing the porosity of the defect layer.
Moreover, for commercial acoustic mirrors which are components of solidly mounted resonators and filters , a low-acoustic-impedance material such as SiO 2 is layered with high-impedance materials such as tungsten or molybdenum. Following Equation 8, for the layer pair of molybdenum and silica, where acoustic impedances are 66.2 MRayl and 13.1 MRayl, respectively, the fixed impedance ratio is 5.1, and the same impedance ratio can be obtained using PS layers of 30 % and 75 %, so, by modulating the porosity, very high reflectivity values can be achieved. Besides, by increasing the number of pairs of layers enclosing the defect layer leads to narrowing of the transmission band together with deepening of the stop band.
We have demonstrated theoretically by using the TMM and experimentally by acoustic transmission measured directly, the formation of acoustic cavity modes in GHz frequencies by introduction of defects into periodic structures based on PS. Acoustic resonances can be tuned at different frequencies by changing the porosity of the defect. And we proved that these resonant modes appear due to the localization of the field into the defect. The acoustic mirrors and cavity structures based on PS have a performance which is at least comparable with that devices based on semiconductor superlattices. This study could be useful for the design of acoustic devices, such as highly selective frequency filters with applications in GHz range.
The authors acknowledge CONACyT for support under project No. 167939.
- Kushwaha MS, Halevi P, Dobrzynski L, Djafari-Rouhani B: Acoustic band structure of periodic elastic composites. Phys Rev Lett 1993, 71: 2022. 10.1103/PhysRevLett.71.2022View Article
- Kushwaha MS, Halevi P, Martínez G: Theory of acoustic band structure of periodic elastic composites. Phys Rev B 1994, 49: 2313. 10.1103/PhysRevB.49.2313View Article
- Sigalas MM, Economou EN: Attenuation of multiple-scattered sound. Europhys Lett 1996, 36: 241. 10.1209/epl/i1996-00216-4View Article
- Kushwaha MS, Halevi P: Giant acoustic stop bands in two-dimensional periodic arrays of liquid cylinders. Appl Phys Lett 1996, 69: 31. 10.1063/1.118108View Article
- Sánchez-Pérez JV, Caballero D, Martínez-Sala R, Rubio C, Sánchez-Dehesa J, Meseguer F, Llinares J, Gálvez F: Sound attenuation by a two-dimensional array of rigid cylinders. Phys Rev Lett 1998, 80: 5325. 10.1103/PhysRevLett.80.5325View Article
- Sigalas MM: Elastic wave band gaps and defect states in two-dimensional composites. J Acoust Soc Am 1997, 101: 1256. 10.1121/1.418156View Article
- Sigalas MM: Defect states of acoustic waves in a two-dimensional lattice of solid cylinders. J Appl Phys 1998, 84: 3026. 10.1063/1.368456View Article
- Kafesaki M, Sigalas MM, Garca N: Frequency modulation in the transmittivity of wave guides in elastic-wave band-gap materials. Phys Rev Lett 2000, 85: 4044. 10.1103/PhysRevLett.85.4044View Article
- Khelif A, Djafari-Rouhani B, Vasseur JO, Deymier PA: Transmission and dispersion relations of perfect and defect-containing waveguide structures in phononic band gap materials. Phys Rev B 2003, 68: 024302.View Article
- Lacharmoise P, Fainstein A, Jusserand B, Thierry-Mieg V: Optical cavity enhancement of light–sound interaction in acoustic phonon cavities. Appl Phys Lett 2004, 84: 3274. 10.1063/1.1734686View Article
- Fokker PA, Dijkhuis JI, de Wijn HW: Stimulated emission of phonons in an acoustical cavity. Phys Rev B 1997, 55: 2925.View Article
- Camps I, Makler SS, Pastawski HM, Foa Torres LEF: GaAs-Al x Ga1−xAs double-barrier heterostructure phonon laser: a full quantum treatment. Phys Rev B 2011, 64: 125311.View Article
- Wu FG, Liu JY, Liu ZY, Liu YY: Splitting and tuning characteristics of the point defect modes in two-dimensional phononic crystals. Phys Rev E 2004, 69: 066609.View Article
- Khelif A, Choujaa A, Benchabane S, Djafari-Rouhani B, Laude V: Guiding and bending of acoustic waves in highly confined phononic crystal waveguides. Appl Phys Lett 2004, 84: 4400. 10.1063/1.1757642View Article
- Psarobas IE, Stefanou N, Modinos A: Phononic crystals with planar defects. Phys Rev B 2000, 62: 5536. 10.1103/PhysRevB.62.5536View Article
- Wang ZG, Lee SH, Kim CK, Park CM, Nahm K, Nikitov SA: Acoustic wave propagation in one-dimensional phononic crystals containing Helmholtz resonators. J Appl Phys 2008, 103: 064907. 10.1063/1.2894914View Article
- Trigo M, Bruchhausen A, Fainstein A, Jusserand B, Thierry-Mieg V: Confinement of acoustical vibrations in a semiconductor planar phonon cavity. Phys Rev Lett 2002, 89: 227402.View Article
- Bisi O, Ossicini S, Pavesi L: Porous silicon: a quantum sponge structure for silicon based optoelectronics. Surf Sci Rep 2000, 38(1–3):5.
- Kiuchi A, Gelloz B, Kojima A, Koshida N: Possible operation of periodically layered nanocrystalline porous silicon as an acoustic band crystal device. In Group-IV Semiconductor Nanostructures: 29 Nov - 2 Dec, Boston Edited by: Tsybeskov L, Lockwood DJ, Delerue C, Ichikawa M. 2004 Materials Research Society Symposia Proceedings Series vol. 832 2005:F371–F376 2004 Materials Research Society Symposia Proceedings Series vol. 832 2005:F371–F376
- Reinhardt A, Snow PA: Theoretical study of acoustic band-gap structures made of porous silicon. Phys Status Solidi A 2007, 204: 15281535.View Article
- Parsons LC, Andrews GT: Observation of hypersonic phononic crystal effects in porous silicon superlattices. Appl Phys Lett 2009, 95: 241909. 10.1063/1.3275742View Article
- Aliev GN, Goller B, Kovalev D, Snow PA: Hypersonic acoustic mirrors and microcavities in porous silicon. Appl Phys Lett 2010, 96: 124101. 10.1063/1.3367747View Article
- Landau LD, Lifshitz M: Theory of Elasticity. Bristol, Pergamon; 1975.
- Ramprasad R, Shi N: Scalability of phononic crystal heterostructures. Appl Phys Lett 2005, 87: 111101. 10.1063/1.2043242View Article
- Phani KK, Niyogi SK, Maitra AK, Roychaudhury M: Strength and elastic modulus of a porous brittle solid: an acousto-ultrasonic study. J Mater Sci 1986, 21: 4335. 10.1007/BF01106552View Article
- Maitra AK, Phani KK: Ultrasonic evaluation of elastic parameters of sintered powder compacts. J Mater Sci 1994, 29: 4415. 10.1007/BF00376263View Article
- Da Fonseca RJM, Saurel JM, Foucaran A, Massone E, Talierco T, Camassel J: Acoustic microscopy invetigation of porous silicon. Thin Solid Films 1995, 225: 155–158.View Article
- Fonseca RJM, Saurel JM, Foucaran A, Camassel J, Massone E, Taliercio T: Acoustic investigation of porous silicon layers. J Mat Sci 1995, 30: 3539. 10.1007/BF00349907View Article
- He J, Sapriel J, Azoulay R: Acoustic attenuation and optical-absorption effects on light scattering by acoustic phonons in superlattices. Phys Rev B 1989, 40: 1121. 10.1103/PhysRevB.40.1121View Article
- Weaver RL: Anomalous diffusivity and localization of classical waves in disordered media: the effect of dissipation. Phys Rev B 1993, 47: 1077. 10.1103/PhysRevB.47.1077View Article
- Liu Z, Zhang X, Mao Y, Zhu YY, Yang Z, Chan CT, Sheng P: Locally resonant sonic materials. Science 2000, 289: 1734–1736. 10.1126/science.289.5485.1734View Article
- Hirsekorn M: Small-size sonic crystals with strong attenuation bands in the audible frequency range. Appl Phys Lett 2004, 84: 3364. 10.1063/1.1723688View Article
- Sainidou R, Stefanou N, Modinos A: Widening of phononic transmission gaps via Anderson localization. Phys Rev Lett 2005, 94: 205503.View Article
- Lanzillotti Kimura ND, Fainstein A, Balseiro CA, Jusserand B: Phonon engineering with acoustic nanocavities: Theoretical considerations on phonon molecules, band structures, and acoustic Bloch oscillations. Phys Rev B 2007, 75: 024301.View Article
- Malpuech G, Kavokin A, Panzarini G, Di Carlo A: Theory of photon Bloch oscillations in photonic crystals. Phys Rev B 2001, 63: 035108.View Article
- Lazcano Z, Arriaga J, Aliev GN: Experimental and theoretical demonstration of acoustic Bloch oscillations in porous silicon structures. J Appl Phys 2014, 115: 154505. 10.1063/1.4871535View Article
- Thönissen M, Berger MG, Billat S, Arens-Fischer R, Krüger M, Lüth H, Theiss W, Hillbrich S, Grosse P, Lerondel G, Frotscher U: Analysis of the depth homogeneity of p-PS by reflectance measurements. Thin Solid Films 1997, 297: 92. 10.1016/S0040-6090(96)09420-5View Article
- Lazcano Z, Arriaga J: High quality porous silicon multilayer structures for infra-red applications. Prog Electromagn Res 2013, 1: 1404.
- Satoh Y, Nishihara T, Yokoyama T, Ueda M, Miyashita T: Development of piezoelectric thin film resonator and its impact on future wireless communication systems. Jpn J Appl Phys 2005, 44: 2883. Part 1 Part 1 10.1143/JJAP.44.2883View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.